Cubic zirconia

From Wikipedia, the free encyclopedia
  (Redirected from DiamondAura)
Jump to: navigation, search
A round brilliant-cut cubic zirconia



Technical aspects[edit]

Cubic zirconia is crystallographically isometric, an important attribute of a would-be diamond simulant. During synthesis zirconium oxide would naturally form monoclinic crystals, its stable form under normal atmospheric conditions. A stabilizer is required for cubic crystals to form, and remain stable at ordinary temperatures; this may be typically either yttrium or calcium oxide, the amount of stabilizer used depending on the many recipes of individual manufacturers. Therefore the physical and optical properties of synthesized CZ vary, all values being ranges.

It is a dense substance, with a specific gravity between 5.6 and 6.0 — at least 1.6 times that of diamond. Cubic zirconia is relatively hard, 8–8.5 on the Mohs scale— slightly harder than most semi-precious natural gems.[1] Its refractive index is high at 2.15–2.18 (compared to 2.42 for diamonds) and its luster is adamantine. Its dispersion is very high at 0.058–0.066, exceeding that of diamond (0.044). Cubic zirconia has no cleavage and exhibits a conchoidal fracture. Because of its high hardness, it is generally considered brittle.

Under shortwave UV cubic zirconia typically fluoresces a yellow, greenish yellow or "beige". Under longwave UV the effect is greatly diminished, with a whitish glow sometimes being seen. Colored stones may show a strong, complex rare earth absorption spectrum.


Discovered in 1892, the yellowish monoclinic mineral baddeleyite is a natural form of zirconium oxide.[2]

The high melting point of zirconia (2750 °C or 4976 °F) hinders controlled growth of single crystals. However, stabilization of cubic zirconium oxide had been realized early on, with the synthetic product stabilized zirconia introduced in 1929. Although cubic, it was in the form of a polycrystalline ceramic: it was used as a refractory material, highly resistant to chemical and thermal attack (up to 2540 °C or 4604 °F).[3]

In 1937, German mineralogists M. V. Stackelberg and K. Chudoba discovered naturally occurring cubic zirconia in the form of microscopic grains included in metamict zircon. This was thought to be a byproduct of the metamictization process, but the two scientists did not think the mineral important enough to give it a formal name. The discovery was confirmed through X-ray diffraction, proving the existence of a natural counterpart to the synthetic product.[4][5]

As with the majority of grown diamond substitutes, the idea of producing single-crystal cubic zirconia arose in the minds of scientists seeking a new and versatile material for use in lasers and other optical applications. Its production eventually exceeded that of earlier synthetics, such as synthetic strontium titanate, synthetic rutile, YAG (yttrium aluminium garnet) and GGG (gadolinium gallium garnet).


Later, Soviet scientists under V. V. Osiko at the Lebedev Physical Institute in Moscow perfected the technique, which was then named skull crucible (an allusion either to the shape of the water-cooled container or to the form of crystals sometimes grown). They named the jewel Fianit after the institute's name FIAN (Physical Institute of the Academy of Science), but the name was not used outside of the USSR. Their breakthrough was published in 1973, and commercial production began in 1976.[6] In 1977 cubic zirconia begun to be mass-produced in the jewelry marketplace.[5] By 1980 annual global production had reached 50 million carats (10 tonnes).

Because the natural form of cubic zirconia is so rare, all cubic zirconia used in jewelry has been synthesized, or created by humans.



The Soviet-perfected skull crucible is still used today, with little variation. Water-filled copper pipes provide a cup-shaped scaffold in which the zirconia feed powder is packed, the entire apparatus being wrapped with radio frequency induction coils running perpendicular to the copper pipes. A stabilizer, typically calcium oxide, is mixed with the feed powder.[3]

The RF induction coils function in a manner similar to the primary winding in a transformer. The zirconia acts as the "secondary winding" of a transformer which in effect is "shorted" out and thus gets hot. This heating method requires the introduction of small pieces of zirconium metal. The metal is placed near the outside of the charge and is melted by the RF coils and heats the surrounding zirconia powder from the outside inwards. The cooling water-filled pipes embracing the outer surface maintain a thin "skin" (1–2 mm) of unmelted feed, creating a self-contained apparatus. After several hours the temperature is reduced in a controlled and gradual manner, resulting in the formation of flawless columnar crystals that are typically about 5 cm long by 2.5 cm wide, although they may be grown much larger. Prolonged annealing at 1400 °C is then carried out to remove any strain. The annealed crystals are then cut into gemstones.[3]

The addition of certain metal oxide dopants into the feed powder results in a variety of colors. For example:

Dopant Color(s)
Cerium yellow
Chromium green
Neodymium purple
Erbium pink
Titanium golden brown


In recent years manufacturers have sought ways of distinguishing their product by supposedly "improving" cubic zirconia. Coating finished CZs in a film of diamond-like carbon (DLC) is one such innovation, a process using chemical vapor deposition. The resulting material is purportedly harder, more lustrous and more like diamond overall. The coating is thought to quench the excess fire of CZ, while improving its refractive index, thus making it appear more like diamond. Additionally, because of the high percentage of diamond bonds in the amorphous diamond coating, the finished simulant will show a positive diamond signature in Raman spectra.

Another technique first applied to quartz and topaz has also been adapted to cubic zirconia: vacuum-sputtering an extremely thin layer of metal oxide (typically gold) on to the finished stones creates an iridescent effect.[7] This material is marketed as "mystic" by many dealers. Unlike DLC, the effect is not permanent, as abrasion easily removes the oxide layer.

Cubic zirconia versus diamond[edit]

There are a few key features of cubic zirconia which distinguish it from diamond:

A triangular facet of a crystal having triangular etch pits with the largest having a base length of about 0.2 mm
  • Hardness: cubic zirconia has a rating of approximately 8 on Mohs hardness scale vs. a rating of 10 for diamond.[1]
  • Dispersion is very high at 0.058–0.066, exceeding a diamond's 0.044.
  • Cut: cubic zirconia gemstones may be cut differently from diamonds. The facet edges can be rounded or "smooth".
  • Color: only the rarest of diamonds are truly colorless, most having a tinge of yellow or brown to some extent. By comparison, a cubic zirconia is often entirely colorless: equivalent to a perfect "D" on diamond's color grading scale. However, some sellers offer near colorless or yellow cubic zirconia, along with other colors, such as pink, green, etc.
  • Thermal conductivity: cubic zirconia is a thermal insulator while diamond is one of the most efficient thermal conductors, with the thermal conductivity exceeding that of most metals. This allows diamond to be distinguished from cubic zirconia with the right instruments.

See also[edit]


  1. ^ a b "Mohs' Hardness of Abrasives". Retrieved 2009-06-06. 
  3. ^ a b c Dhanaraj, Govindhan; Byrappa, Kullaiah and Prasad, Vishwanath (2010). Springer Handbook of Crystal Growth. Springer. pp. 443–. ISBN 978-3-540-74761-1. Retrieved 1 February 2013. 
  4. ^ Stackelberg, M. von and Chudoba, K. (1937). "Dichte und Struktur des Zirkons; II". Zeitschr. Kristallographie 97: 252–262. 
  5. ^ a b "Understanding more about Cubic Zirconia". Chic Jewelry. 2013. Retrieved 6 December 2013. 
  6. ^ Hesse, Rayner W. Jewelrymaking Through History: An Encyclopedia. Greenwood Publishing Group. p. 72. ISBN 978-0-313-33507-5. 
  7. ^ "Designer Enhanced Gemstones". Azotic Coating Technology, Inc. 2010. Retrieved 3 November 2010. 

Further reading[edit]